Photoelectrochemical Performance of Quantum dot-Sensitized TiO2 Nanotube Arrays: a Study of Surface Modification by Atomic Layer Deposition Coating
© The Author(s). 2017
Received: 31 December 2016
Accepted: 29 March 2017
Published: 7 April 2017
Although CdS and PbS quantum dot-sensitized TiO2 nanotube arrays (TNTAs/QDs) show photocatalytic activity in the visible-light region, the low internal quantum efficiency and the slow interfacial hole transfer rate limit their applications. This work modified the surface of the TNTAs/QDs photoelectrodes with metal-oxide overlayers by atomic layer deposition (ALD), such as coating Al2O3, TiO2, and ZnO. The ALD deposition of all these overlayers can apparently enhance the photoelectrochemical performance of the TNTAs/QDs. Under simulated solar illumination, the maximum photocurrent densities of the TNTAs/QDs with 10 cycles ZnO, 25 cycles TiO2, and 30 cycles Al2O3 overlayers are 5.0, 4.3, and 5.6 mA/cm2 at 1.0 V (vs. SCE), respectively. The photoelectrode with Al2O3 overlayer coating presents the superior performance, whose photocurrent density is 37 times and 1.6 times higher than those of the TNTAs and TNTAs/QDs, respectively. Systematic examination of the effects of various metal-oxide overlayers on the photoelectrochemical performance indicates that the enhancement by TiO2 and ZnO overcoatings can only ascribed to the decrease of the interfacial charge transfer impedance, besides which Al2O3 coating can passivate the surface states and facilitate the charge transfer kinetics. These results could be helpful to develop high-performance photoelectrodes in the photoelectrochemical applications.
TiO2 is a kind of inorganic semiconductor materials with excellent photocatalytic activity, non-toxicity, and good stability. It is widely used in the fields of water splitting, photocatalysis, solar cells, lithium ion battery, etc. In 1972, Honda and Fujishima have achieved water splitting using TiO2 photoanode under xenon lamp irradiation . Different architectures of TiO2 nanomaterials have been fabricated, such as nanoparticles , nanowires , nanotubes , nanosheets , nanoflowers , hollow spheres  etc. Especially the nanotube arrays have been widely studied with excellent optical excitation and charge transfer properties. However, TiO2 cannot effectively use the visible light because of its wide bandgap (∼3.2 eV). Transition metals  or nonmetals  doping can reduce the bandgap of TiO2, but the dopants can easily become the electron-hole recombination centers . The other method is using narrow-bandgap materials such as quantum dots (QDs) to sensitize TiO2 and enhance their photocatalytic activity in the visible-light region since the photogenerated charge can quickly separate and transfer between different semiconductors [11, 12]. CdS , CdSe , PbS , and PbSe  quantum dots can respond to the visible light with a tunable bandgap . In recent years, co-sensitized TiO2 with quantum dots such as CdSe/CdTe , CdS/CdSe , and PbS/CdS  have been reported. However, the efficiency of quantum dot-sensitized TiO2 photoelectrodes is still at a lower level. The main reasons are the serious optical etching and the large number of defects in the surface of the quantum dots which will lead to the formation of charge recombination centers.
Surface modification by atomic layer deposition (ALD) is an advanced method to prepare metal-oxide layers on the electrodes to improve their performance. Al2O3, TiO2, and ZnO are three kinds of common metal oxides which could be prepared by ALD for surface modification. The process is that two precursors are separately introduced into the reaction chamber by alternation pulse, and the chemical adsorption and surface reaction will occur on the sample . Compared with traditional deposition methods, ALD can prepare uniform and controllable thin film. Metal oxides prepared by ALD technique have been used to passivate surface defects of semiconductor materials in the fields of photocatalysis and water splitting. For photoelectrochemical water splitting, ALD technique has been employed and showed promising results for Al2O3/TiO2 , TiO2/TiO2 nanorod arrays , ZnO/TiO2 [24, 25], and Co3O4/TiO2 . In the previous reports, however, such metal-oxide layers were mostly used as an energy barrier between quantum dots sensitizer and semiconductor electrodes to suppress charge recombination and improve the incorporated amounts of QDs. There are still few systematic studies on the effects of metal-oxide overlayers on the photoelectrochemical performance of the QD-sensitized photoelectrodes, and even no comprehensive comparison of Al2O3, TiO2, and ZnO has been reported so far. However, such information is not only significant to understand the various underlying mechanisms of the different overcoatings but also valuable for proper selection of metal-oxide overlayer to improve the photoelectric properties and for rational design and optimization of high-performance photoelectrodes.
We report here the improving photoelectrochemical performance of quantum dot-co-sensitized TiO2 nanotube arrays through surface modification by ALD coating various metal-oxide overlayers. The CdS and PbS quantum dot-co-sensitized TNTA photoelectrode shows a significant enhancement in the visible-light absorption range between 400 and 600 nm. Three kinds of metal-oxide overlayers, Al2O3, TiO2, and ZnO, have been uniformly coated throughout the surface of the photoelectrodes by ALD. Their photoelectrochemical performance has been studied by linear sweep voltammetry, electrochemical impedance spectroscopy, and Mott-Schottky analysis. The systematic examination of the role of various metal-oxide overlayers reveals the underlying mechanism of the enhancement. The results show that ALD deposition of metal-oxide overlayers is a promising and facile method to improve the photoelectric properties of the semiconductor electrodes.
Preparation of TiO2 Nanotube Arrays
Prior to electrochemical anodization, Ti foils with a thickness of 0.5 mm and purity of 99.5% were chemical polished and ultrasonically cleaned in acetone, ethanol, and deionized water (DI) for 15 min successively. TNTAs were prepared by anodic oxidation method in a two-electrode system with titanium plates as working electrode and stainless steel sheet as counter electrode. The electrolyte was 0.27 M NH4F solution, and the solvent was a mixture of glycerin and DI water with the volume ratio of 1:1. The anodic oxidation was conducted at a biased of 25 V for 5 h at room temperature . After the oxidation, the TNTAs obtained were soaked in ethanol for 3 min ultrasonic cleaning in order to remove the white floc surface. In order to convert amorphous structures to the crystalline phase, the samples were annealed at 450 °C for 3 h and 45 min with a heating rate of 2 °C/min, and then heat cooled to room temperature in the furnace.
Preparation of CdS/PbS Co-sensitized TiO2 Nanotube Arrays
PbS and CdS quantum dots were loaded over crystallized TiO2 nanotube arrays by the successive ionic layer adsorption and reaction (SILAR) method. The specific steps are as follows: The precursor solutions were 0.02 M Pb (NO3)2 methanol solution and 0.02 M Na2S solution of methanol and deionized water (V:V = 1:1). TNTAs were first dipped in 0.02 M Pb (NO3)2 methanol solution for 15 s, and then keep for 1 min 45 s, rinsed with methanol, dipped in 0.02 M Na2S solution for 15 s, and then keep for 1 min 45 s rinsed with methanol; two procedures were termed as one deposition cycle of PbS quantum dots and then repeated 5 times. Secondly, the samples were sensitized with CdS quantum dots immediately. Similar to the procedure above, the deposition cycles of CdS quantum dots were 5 as well. The precursor solutions were 0.05 M Cd (NO3)2 ethanol solution and 0.05 M Na2S solution (volume ratio of methanol and DI water is 1:1). The sample is referred to as TNTAs/QDs . Finally, the sample was covered with 2 cycles ZnS protecting layer to reduce surface recombination [28, 29].
Preparation of TiO2 Co-sensitized CdS/PbS Nanotube Arrays Modified by ALD Metal Oxide Overlayers
ALD method was then applied for metal-oxide overlayer coating. In order to guarantee that the photogenerated electrons can tunnel through the overlayer and the results are comparable, the overlayer thickness is kept about 1.5 nm. This requires the overlayer deposition with 30 cycles Al2O3 (0.5 Å/cycle), 25 cycles TiO2 (0.6 Å/cycle), and 10 cycles ZnO (1.5 Å/cycle), respectively. The precursor was dissolved in 1 M heptane in solution, the reactor temperature is 150 °C, and N2 as carrier gas and washing gas. For Al2O3 deposition, three methyl aluminum (trimethylaluminum, TMA) was used as precursor. The specific steps are as follows. TNTAs/QDs samples were first put in the chamber. An ALD cycle of Al2O3 deposition consisted of a 0.02 s pulse of TMA, 5 s exposure to TMA, 15 s purge with N2 and then 0.05 s pulse of H2O, 5 s exposure to H2O, final 15 s purge with N2, thus completing a cycle of Al2O3 deposition . An ALD cycle of TiO2 deposition and ZnO deposition were similar to the above procedures but selected diethyl zinc (DEZ) and titanium (IV) isopropoxide as their precursors, respectively . In order to minimize the effect of surface area variation, we carefully controlled the process condition for preparing the quantum dot-sensitized TiO2 nanotube arrays and kept the thickness of the passivation layer deposited as about 1.5 nm.
Characterization and Photoelectrochemical Performance Testing
The surface morphology and microstructure of the samples were observed by using scanning electron microscopy (FESEM, Hitachi, S4800) and transmission electron microscopy (TEM, JEM 2100). Energy dispersive X-ray spectrometer (EDS) accompanying FESEM was used to analyze sample element. X-ray diffraction (XRD, Bruker D8) with Cu Ka radiation was used to analyze the crystal structure of the samples. The optical absorption properties of the samples were recorded by UV-Vis spectrophotometer (UV, Purkinje TU-1901).
The photoelectric properties of the samples were tested by electrochemical workstation (Zennium Zahner) in a standard three-electrode setup with the prepared sample as the working electrode with a specific exposure area of 1 cm2. A double salt bridge saturated calomel electrode (SCE) and a Pt wire were the reference and the counter electrodes, respectively. The electrolyte was a aqueous solution mixed with 0.1 M Na2S and 0.2 M Na2SO3 with a volume ratio of 1:1 (pH = 12.2). The voltage scan rate of linear sweep voltammetry (LSV) test was 10 mV/s, and the excitation light source was a 500 W xenon lamp with the wavelength range from 350 to 1100 nm and calibrated through an AM 1.5 filter and PC-2 solar radiation recorder (AM 1.5G, 100 mW/cm2). LED lamp was used as the excitation light source of the transient photocurrent test with electrochemical workstation (wavelength 565 + 112 nm; light intensity 80 mW/cm2), while every 25 s for a range of switch lamp to achieve light and dark conditions.
Electrochemical impedance spectroscopy (EIS) was examined under open-circuit voltage and simulated solar light condition. The amplitude was 10 mV and the frequency range was from 0.1 Hz to 100 KHz. Mott-Schottky analysis was performed in the dark condition, and the voltage range is from −1 to 0.9 V. The scanning rate was 30 mV/s, and the frequency and amplitude perturbation were 1 kHz and 10 mV.
Results and Discussion
Atomic percentages of the elements derived in EDS spectra
0 cycles [%]
30 cycles Al2O3 [%]
25 cycles TiO2 [%]
10 cycles ZnO [%]
The photoconversion efficiency of each electrode under different bias voltages is shown in Fig. 6b. The maximum photoconversion efficiencies of the TNTAs, TNTAs/QDs, TNTAs/QDs/10 cycles ZnO, TNTAs/QDs/25 cycles TiO2, and TNTAs/QDs/30 cycles Al2O3 electrodes are 0.06, 2.57, 3.95, 3.41, and 4.23% respectively. Thus, deposition of the metal-oxide layers onto the TNTA/QD photoelectrode can apparently increase their photoconversion efficiency. The efficiency of TNTAs/QDs/30 cycles Al2O3 is 1.6 times as much as TNTAs/QDs, better than the other photoelectrode. Compared with the TNTAs, the photoconversion efficiency could be maximally increased by 41 times after QDs co-sensitization and metal-oxide overlayer deposition.
Figure 6c presents the transient light response of the TNTA/QD electrodes with different ALD overlayers under the white-light excitation with the density of 80 mW/cm2 and the wavelength range of 565 ± 112 nm. The photocurrent of the four samples increased rapidly with the switching on of the LED lamp, which indicates that the photogenerated electrons in the electrode can rapidly be excited and injected into the TNTAs from the quantum dots. The photocurrent density of each electrode recorded after the five switch lamp cycles shows no significant decrease which suggests the stability of the electrodes.
EIS results in Fig. 7a qualitatively demonstrate the charge transfer properties of the photoelectrodes with and without oxide passivation layer. The interfacial charge transfer impedance is inversely proportional to the arc diameters in the Nyquist plots. Among the four photoelectrodes, the interfacial charge transfer impedance increases as the following trend: TNTAs/QDs/30 cycles Al2O3, TNTAs/QDs/10 cycles ZnO, TNTAs/QDs/25 cycles TiO2, and TNTAs/QDs. It can be seen that all the oxide layers can reduce the interfacial charge transfer impedance, which will accelerate the carrier separation and transmission and then improve the photoelectrochemical performance. From the Mott-Schottky measurements in Fig. 7b, the carrier concentrations of the TNTAs/QDs, TNTAs/QDs/10 cycles ZnO, and TNTAs/QDs/25 cycles TiO2 electrodes could be calculated as 3.36 × 1019 cm−3, while the TNTAs/QDs/30 cycles Al2O3 electrode is 1.32 × 1020 cm−3. The charge carriers are generated in a semiconductor by the irradiation with light energy larger than its bandgap. There are a large number of defects on the surface of the TNTA/QD electrode. These defects work as recombination centers, leading to a decrease in carrier concentration. The Al2O3 layer coating on the surface of quantum dots plays a key role to passivate the surface defects and reduce charge recombination. Thus, Al2O3 coating can be found to increase the effective carrier concentration. In addition, when the electrode deposited with the Al2O3 passivation layer is exposed to light, the photogenerated holes in the valence band are rapidly injected from the quantum dots into the quantum dot/Al2O3 interface under the built-in electric field. Moreover, the negative charge in the Al2O3 layer would form a built-in electric field which can prevent the photogenerated electrons inside the bulk material, thus effectively reduce the recombination of photogenerated charges . Although the surface passivation effect on TiO2 nanorod arrays with TiO2 coating were reported in the literature , according to our Mott-Schottky results, the carrier concentrations of the TNTA/QD electrode with TiO2 and ZnO coating keep the same as that of the TNTAs/QDs electrode, indicates that TiO2 and ZnO overlayers can hardly passivate the surface defects of the TNTAs/QDs electrode. The enhancement by TiO2 and ZnO overcoating is mainly due to the reduction of the interfacial charge transfer impedance.
The photochemical stability of the photoanodes is another important concern. After a series of electrochemical performance tests (transient photocurrent, LSV, and EIS tests) under illumination, there were no evident changes in photoelectrochemical performance for the three samples. But under 2 h continuous illumination, the photocurrent density of the photoelectrode with 30 cycles Al2O3 decayed slowly while that of the bare electrode suffered serious decay. This is because Al2O3 oxide layer has been partially dissolved in the electrolyte (a mixed solution of Na2SO3 and Na2S, used to prevent the oxidation of sulfide ions), leading to decrease of the transformation of photogenerated electrons and holes. The photochemical stability of the photoelectrodes with the ZnO and TiO2 overlayers shows similar decay to that with Al2O3, which is possibly due to their similar amorphous nature. In terms of long-term photochemical stability, future work is required to understand the underlying reason and to optimize the overlayer by improving the crystallinity or combining different oxide layers by ALD.
ALD technology has been applied to deposit various uniform and compact oxide overlayers, Al2O3, TiO2, and ZnO with controllable thickness, on the TNTAs/QDs structure. These overlayers within the tunneling thickness of approximately 1.5 nm can enhance the photoelectric properties of the TNTA/QD photoelectrodes. Under simulated sunlight, the maximal photocurrent densities of the TNTAs/QDs with 10 cycles ZnO, 25 cycles TiO2, and 30 cycles Al2O3 overlayers are 5.0, 4.3, and 5.6 mA/cm2, respectively. All the three oxide overcoating can improve the photoelectrochemical performance of the TNTAs/QDs, but the underlying mechanisms are different. Al2O3 overlayer can chemically passivate the surface defects of the TNTA/QDs electrode, reduce the charge recombination, and improve the transfer efficiency of the charge in the bulk material and the transfer kinetics at the interface. This leads to the superior performance than TiO2 and ZnO overlayers, which just reduce the interfacial charge transfer impedance in varying degrees without increasing the carrier concentration. This work demonstrates that the proper selection of metal-oxide overlayer is of great importance to improve the photoelectric properties, and the ALD technology is a promising and facile method for surface modification to prepare the high-performance electrodes in the photoelectrochemical applications.
This work is supported by the National Natural Science Foundation of China (Grant No. 51462008), National High Technology Research and Development Program of China (863 Program, Grant No. 2015AA034103), and Innovative Research Team Project of Natural Science Foundation of Hainan Province (Grant No. 2016CXTD001).
QZ designed and conducted the experiments and analyses and drafted the manuscript. JZ and MZ provided the technical support and conceptual advice. GW and YC participated in the design of the study. SL conceived the idea and modified the manuscript. All authors read and approved the final manuscript.
The authors declare that they have no competing interests.
Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
Open AccessThis article is distributed under the terms of the Creative Commons Attribution 4.0 International License (http://creativecommons.org/licenses/by/4.0/), which permits unrestricted use, distribution, and reproduction in any medium, provided you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made.
- Fujishima A, Honda K (1972) TiO2 photoelectrochemistry and photocatalysis. Nature 238:37–38View ArticleGoogle Scholar
- Burnside SD, Shklover V, Barbé C, Comte P, Arendse F, Brooks K, Grätzel M (1998) Self-organization of TiO2 nanoparticles in thin films. Chem Mater 10:2419–2425View ArticleGoogle Scholar
- Lin Y, Wu GS, Yuan XY, Xie T, Zhang LD (2003) Fabrication and optical properties of TiO2 nanowire arrays made by sol–gel electrophoresis deposition into anodic alumina membranes. J Phys Condens Matter 15:2917View ArticleGoogle Scholar
- Zhu K, Neale NR, Miedaner A, Frank AJ (2007) Enhanced charge-collection efficiencies and light scattering in dye-sensitized solar cells using oriented TiO2 nanotubes arrays. Nano Lett 7:69–74View ArticleGoogle Scholar
- Yu J, Qi L, Jaroniec M (2010) Hydrogen production by photocatalytic water splitting over Pt/TiO2 nanosheets with exposed (001) facets. J Phys Chem C 114:13118–13125View ArticleGoogle Scholar
- Zhang M, Shao C, Guo Z, Zhang Z, Mu J, Cao T, Liu Y (2011) Hierarchical nanostructures of copper (II) phthalocyanine on electrospun TiO2 nanofibers: controllable solvothermal-fabrication and enhanced visible photocatalytic properties. ACS Appl Mater Interfaces 3:369–377View ArticleGoogle Scholar
- Xuan S, Jiang W, Gong X, Hu Y, Chen Z (2008) Magnetically separable Fe3O4/TiO2 hollow spheres: fabrication and photocatalytic activity. J Phys Chem C 113:553–558View ArticleGoogle Scholar
- Martins PM, Gomez V, Lopes AC, Tavares CJ, Botelho G, Irusta S, Lanceros-Mendez S (2014) Improving photocatalytic performance and recyclability by development of Er-doped and Er/Pr-codoped TiO2/poly (vinylidene difluoride)–trifluoroethylene composite membranes. J Phys Chem C 118:27944–27953View ArticleGoogle Scholar
- Sakthivel S, Kisch H (2003) Daylight photocatalysis by carbon-modified titanium dioxide. Angew Chem Int Ed 42:4908–4911View ArticleGoogle Scholar
- Li GS, Zhang DQ, Yu JC (2009) A new visible-light photocatalyst: CdS quantum dots embedded mesoporous TiO2. Environ Sci Technol 43:7079–7085View ArticleGoogle Scholar
- Zhang X, Lin S, Liao J, Pan N, Li D, Cao X, Li J (2013) Uniform deposition of water-soluble CdS quantum dots on TiO2 nanotube arrays by cyclic voltammetric electrodeposition: Effectively prevent aggregation and enhance visible-light photocatalytic activity. Electrochim Acta 108:296–303Google Scholar
- Hensel J, Wang G, Li Y, Zhang JZ (2010) Synergistic effect of CdSe quantum dot sensitization and nitrogen doping of TiO2 nanostructures for photoelectrochemical solar hydrogen generation. Nano Lett 10:478–483View ArticleGoogle Scholar
- Sun WT, Yu Y, Pan HY, Gao XF, Chen Q, Peng LM (2008) CdS quantum dots sensitized TiO2 nanotube-array photoelectrodes. J Am Ceram Soc 130:1124–1125Google Scholar
- Lee YL, Huang BM, Chien HT (2008) Highly efficient CdSe-sensitized TiO2 photoelectrode for quantum-dot-sensitized solar cell applications. Chem Mater 20:6903–6905View ArticleGoogle Scholar
- Hoyer P, Könenkamp R (1995) Photoconduction in porous TiO2 sensitized by PbS quantum dots. Appl Phys Lett 66:349–351View ArticleGoogle Scholar
- Pietryga JM, Schaller RD, Werder D, Stewart MH, Klimov VI, Hollingsworth JA (2014) Pushing the band gap envelope: mid-infrared emitting colloidal PbSe quantum dots. J Am Chem Soc 126:11752–11753View ArticleGoogle Scholar
- Kim JC, Choi J, Lee YB, Hong JH, Lee JI, Yang JW, Lee WI, Hur NH (2006) Enhanced photocatalytic activity in composites of TiO2 nanotubes and CdS nanoparticles. Chem Commun 48:5024–5026Google Scholar
- de Mello DC, Koole R (2009) Size dependence of the spontaneous emission rate and absorption cross section of CdSe and CdTe quantum dots. J Phys Chem C 113:6511–6520Google Scholar
- Lee YL, Chi CF, Liau SY (2009) CdS/CdSe co-sensitized TiO2 photoelectrode for efficient hydrogen generation in a photoelectrochemical cell†. Chem Mater 22:922–927View ArticleGoogle Scholar
- Lv P, Fu W, Mu Y, Sun H, Su S, Chen Y, Yang H (2015) Photoelectrochemical property of CdS and PbS cosensitized on the TiO2 array by novel successive ionic layer adsorption and reaction method. J Alloys Compd 621:30–34View ArticleGoogle Scholar
- George SM (2008) Atomic layer deposition: an overview. Chem Rev 110:111–131View ArticleGoogle Scholar
- Roelofs KE, Brennan TP, Dominguez JC, Bailie CD, Margulis GY, Hoke ET, Bent SF (2013) Effect of Al2O3 recombination barrier layers deposited by atomic layer deposition in solid-state CdS quantum dot-sensitized solar cells. J Phys Chem C 117:5584–5592View ArticleGoogle Scholar
- Mali SS, Shim CS, Park HK, Heo J, Patil PS, Hong CK (2015) Ultrathin atomic layer deposited TiO2 for surface passivation of hydrothermally grown 1D TiO2 nanorod arrays for efficient solid-state perovskite solar cells. Chem Mater 27:1541–1551View ArticleGoogle Scholar
- Kao MC, Chen HZ, Young SL (2009) Effects of ZnO coating on the performance of TiO2 nanostructured thin films for dye-sensitized solar cells. Appl Phys A 97:469–474View ArticleGoogle Scholar
- Lee W, Kang SH, Kim JY, Kolekar GB, Sung YE, Han SH (2009) TiO2 nanotubes with a ZnO thin energy barrier for improved current efficiency of CdSe quantum-dot-sensitized solar cells. Nanotechnology 20:335706View ArticleGoogle Scholar
- Huang B, Yang W, Wen Y, Shan B, Chen R (2014) Co3O4-modified TiO2 nanotube arrays via atomic layer deposition for improved visible-light photoelectrochemical performance. ACS Appl Mater Interfaces 7:422–431View ArticleGoogle Scholar
- Li D, Lin S, Li S, Huang X, Cao X, Li J (2012) Effects of geometric and crystal structures on the photoelectrical properties of highly ordered TiO2 nanotube arrays. J Mater Res 27:1029–1036View ArticleGoogle Scholar
- Zhang X, Zeng M, Zhang J, Song A, Lin S (2016) Improving photoelectrochemical performance of highly-ordered TiO2 nanotube arrays with cosensitization of PbS and CdS quantum dots. RSC Adv 6:8118–8126View ArticleGoogle Scholar
- Kim HJ, Lee HD, Kumar CSSP, Rao SS, Chung SH, Punnoose D (2015) The effect of manganese in a CdS/PbS colloidal quantum dot sensitized TiO2 solar cell to enhance its efficiency. New J Chem 39:4805–4813View ArticleGoogle Scholar
- Zeng M, Peng X, Liao J, Wang G, Li Y, Li J, Lin S (2016) Enhanced photoelectrochemical performance of quantum dot-sensitized TiO2 nanotube arrays with Al2O3 overcoating by atomic layer deposition. Phys Chem Chem Phys 18:17404–17413View ArticleGoogle Scholar
- Zeng M, Zeng X, Peng X, Zhu Z, Liao J, Liu K, Lin S (2016) Improving photoelectrochemical performance on quantum dots co-sensitized TiO2 nanotube arrays using ZnO energy barrier by atomic layer deposition. Appl Surf Sci 388:352–358View ArticleGoogle Scholar
- Hwang YJ, Hahn C, Liu B, Yang P (2012) Photoelectrochemical properties of TiO2 nanowire arrays: a study of the dependence on length and atomic layer deposition coating. ACS Nano 6:5060–5069View ArticleGoogle Scholar